## For Peer Review

Geometric modelling of 3D woven preforms in composite

T-joints

Journal: *Textile Research Journal*

Manuscript ID TRJ-17-0023.R1 Manuscript Type: Original Manuscript

Keywords: weaving < Fabrication, Fabrication < Fabrication, processing < Fabrication, composites < Materials

Abstract:

A common method to fabricate net-shaped 3D woven preforms for composite T-joints is to weave flat 3D preforms via a standard weaving machine with variation in binder yarn path and then separate the preform in the form of a bifurcation. Folding introduces fibre architecture

deformation at the 3D woven bifurcation area. In this paper, a geometric modelling approach is proposed to represent the realistic fibre architecture, as a preprocessor for finite element analyses to predict composite

structural performance. Supported by x-ray micro-computed tomography (µCT), three important deformation mechanisms are observed including yarn stack shifting, cross-section bending and cross-section flattening resulting from the folding process. Furthermore, a set of mathematical formulae for simulation of the deformations in the junction region are developed and satisfactory agreement is observed when compared with µCT scan results.

## For Peer Review

**Nomenclature**

- height of warp yarn

- height of weft yarn

- width of warp yarn

- width of weft yarn

- spacing of weft yarns between through-thickness layers

– spacing of warp yarn in the same layer

- radius of curvature of centreline of warp yarn cross-section on yarn layer *n*(µCT measurement)

_{ - radius of curvature of centreline of weft yarn layer }_{n}_{(µCT measurement)}

- radius of curvature of centreline of warp yarn cross-section on yarn layer *n*(calculated)

- radius of curvature of centreline of weft yarn layer *n*(calculated)

– radius of compaction mould fillet

- maximum width of the cross-sectional gap in a flattened weft yarn

- warp yarn angle shit

- warp yarn displacement shit

- offset distance from the centre of nearest unbent weft yarn

*d* - distance from a specific fibre layer within the yarn to the reference fibre layer

- the maximum value of *d *

- arc length difference between fibre on a specific fibre layer, distance *d* away from reference fibre
layer, and fibre on reference layer

- radius of curvature of the reference fibre within a bent yarn

- radius of curvature of the fibre that is distance *d* away from the reference fibre within a bent yarn

*α* - a proportion of arc length difference _{}

- the values of *α *for the ideally migrated fibres

### Field Code Changed

**Field Code Changed**

**Field Code Changed**

## For Peer Review

*LABCD* - the arc length of fibre ABCD

- length of yarn width transition

- displacement of out-of-plane fibre migration

displacement of out-of-plane migration for fibre on fibre layer *k* within a yarn

- length of line AB

- length of arc AB

!" - total fibre area in yarn extension

- fibre diameter

*nf* - the number of total fibre layers along the yarn height direction before flattening

*ext*
*weft*

*W* - weft yarn width extension

*fla*
*weft*

*H* - flattened height of weft yarn

*fla*
*weft*

*W* - flattened width of weft yarn

## Introduction

3D woven composites are reinforced by 3D woven preforms containing yarns in *x*, *y* and *z* directions. 3D

woven preforms, specifically for composite applications, are generally classified into orthogonal,

through-the-thickness angle interlock and layer-to-layer angle interlock patterns. Design and manufacturing of

emerging multi-axis 3D woven preforms incorporating bias yarn layers has also been proposed but the

development is still at an early stage for applications.1_{ 3D woven composites have drawn great attention in }

recent decades for their advantages such as higher through-thickness properties that can help to overcome

the problem of delamination encountered by 2D laminates.1_{ The exploration of 3D reinforced composites }

has been also extended to load-bearing profiles like T, I, and Pi shaped joints. There are three basic ways to

manufacture 3D reinforced composite joints with woven preforms. The first method is to use 2D woven

fabric lay-ups, reinforcing the through-thickness direction with stitching or Z-pinning.2,3 The second way is

to weave flat 3D preforms via a standard weaving machine with variation of binder yarn path to form

locally unreinforced planes (bifurcations) and then fold the preforms into the desired shape.4-7_{ The third }

**Formatted:** Font color: Red

## For Peer Review

way is to fabricate the preform directly into a complex 3D shape through a specially developed 3D weaving

loom.8-10 Although composites reinforced by the first method can offer better damage tolerance in terms of

delamination than 2D laminated joints subjected to equivalent loads,2,11 they can be less competitive in

in-plane properties because of geometric defects or fibre damage caused by retrospectively inserting

through-thickness reinforcements.12_{ In addition, due to the high investment and innovation needed for developing a }

special 3D loom for the third kind of preform, 3D preforms woven by a conventional loom are popular for

current composite T-joints.

## 3D woven

type 1

3D woven

type 2

1 2 3 4 5 4'(5') 3' 2' 1' 5 4 3 2 1 1' 2' 3' 4' 5' 1 2 3 4 5 4'(5') 3' 2' 1'

1 2 3 4 5 1' 2' 3' 4' 5'

1 2 3 4 5 1 2 3 4 5 4'(5' ) 3' 2' 1' 5' 4' 3' 2' 1' 1 2 3 4 5 4'(5') 3' 2' 1'

1 2 3 4 5

1' 2' 3' 4' 5'

[image:4.612.83.444.243.582.2]warp

weft

Figure 1. Top, load-displacement curves for the two types of 3D woven composite T-joints in comparison with an equivalent 2D twill woven T-joint16; bottom, schematic woven structures for the T-joints showing weave variation in the noodle regionat the junction(dashed line area), with binders omitted

However, deformation is likely to occur when folding a flat woven preform into a 3D shape. Because the

internal architecture of a woven preform is complex, its variability in geometry can directly affect material

properties such as permeability and formability.13,14 At the micro-scale, the fibre misalignment in fibre

**Formatted:** Font: 10 pt, Font color: Red

## For Peer Review

bundles was also found to have an influence on many aspects of composite behaviour.15_{ Previous studies }

have also shown that reinforcement geometry plays an important role in determining the composite’s

mechanical properties, as two types of 3D woven composite T-joints with only weave variation at the 3D

woven bifurcation area (in which the formed resin pocket is usually referred to as the ‘noodle’) were tested

under the same tensile loading case but very different load-displacement responses were observed

(Figure.1).16_{ Thus, in order to closely predict the properties of composite T-joints reinforced by a flat }

woven 3D preform, it is necessary to model the fibre architecture as realistically as possible.

Characterising the realistic fibre architecture of 3D woven composites is difficult because of the complexity

of the internal geometry, but this can benefit from the use of x-ray micro-Computer Tomography

(µCT).17,18 Some general frameworks for geometric modelling of woven preforms with respect to

characterisation of yarn path, crimp and cross-section shape have been provided in the literature.19-22

Furthermore, compaction induced yarn crimp and cross-section shape change were studied with a number

of models,23,24_{ however, as they are based on beam theory, numerically solved by the finite element }

method, they are computationally intensive. Some mathematical methods were also proposed to model yarn

cross-section shape under compression. An energy based method used to characterise yarn deformation in

compression was developed by Lomov and Verpoest25 but the method asks for a measurement of the

mechanical properties of yarns in bending and compression. Chen et.al26,27 modelled yarn cross-section

deformation of both single and multi-layer woven preforms under compaction at the mesoscopic level

based on the assumption that yarn width deformation is negligible compared with the deformation of yarn

thickness. The model is not applicable when yarn width change is significant, for instance for a yarn

subjected to bending load. Cornelissen and Akkerman28 observed yarn cross-section flattening in a

cantilever experiment of yarns bending under their own weight. They concluded that cross-section

flattening would affect the yarn flexural rigidity by one order of magnitude but they were not able to derive

a trend from the experiment. However, yarn cross-section deformation in bending is significant as observed

in this study via µCT analysis and an effective model is needed to capture this feature.

This paper focuses on the geometric modelling of 3D woven preform deformation caused by folding a flat

woven preform into a T-piece, which is a typical fabrication process for composite T-joints. Through the

µCT analysis of a compacted preform, three important deformation mechanisms specifically for this type of

7

## For Peer Review

preform were observed, namely yarn stack shifting, cross-section bending and cross-section flattening

resulting from the folding process. These features have been geometrically modelled and the models have

been validated against µCT analysis data of a 3D woven T-joint preform.

Material characterisation

The example preform reinforcing the composite T-joints is a 3D orthogonal weave provided by Sigmatex,

UK based on Hexcel IM7 12K carbon fibre, which is woven flat on a Jacquard machine and folded into a T

shape. 3D orthogonal weaves are 3D structures containing straight warp and weft yarns in the *x*, *y*

directions and binders (also called ‘warp weavers’) that interlace with other yarns, at times, orientated in

the through-thickness direction, providing high stiffness under tensile loading due to low yarn waviness.10

The preform consists of 8 layers of warp yarns and 9 layers of weft yarns in the web, and 4 layers of warp

yarns and 5 layers of weft yarns in the flange. A schematic woven structure for this preform before and

after bifurcation is shown as ‘3D woven type 1’ in Figure 1.

To characterize the intrinsic geometric features of this type of preform for composite T-joints, the dry

preform was compacted into a T-shape acrylic fixture and analysed via µCT as shown in Figure 2. The web

section of the preform was firstly fitted in the fixture before bifurcation of the flange section, thus no

deformation in the web is likely to be expected from preform bifurcation and the part of the preform

contacting the fixture corner would conform to its radius of curvature. The GE phoenix v|tome|x m machine

used a current of 240 µA and a voltage of 120 kV to achieve the imaging resolution of 30 µm per pixel in

scanning. The compaction leads to an average fibre volume fraction of 45% which is calculated based on

the preform areal weight with 4mm thickness in the web and 2mm in the flange. The preform has two

geometric changes in its left-hand side: one is that the warp yarns at the junction (curved region) are in

twice the filament count as those in the web; the other is a weft layer in the web (numbered as 4'(5') in

Figure 2) is formed of twofold weft yarns as used in other layers and separated into two layers (layer 4' and

5') at the flange, for the purpose of yarn layer balance in the flange. Meanwhile, the flange part of the

preform was woven with warp yarns of 24k filament count.

**Formatted:** Font color: Red

**Formatted:** Font color: Red

**Formatted:** Font color: Red

## For Peer Review

Figure 2. µCT scan of the preform: (a) preform visualised via volume rendering from µCT showing the yarn directions; (b) schematic 3D orthogonal weave pattern (created by TexGen) ; (c) µCT section view of the preform with the numbers showing the numbering of weft layers

In order to validate the proposed geometric modelling approach, necessary geometric parameters measured

from the preform are listed in Table 1. In addition, the intra-yarn fibre volume fractions at different

locations inferred from the cross-sectional data were given, assuming a rectangular cross-section for the

yarns. Measurements of each parameter were made using the software ImageJ at a number of µCT slices

covering different yarns, from which the average and standard deviation (SD) were obtained. The folding

process introduces additional yarn deformation at the junction, and three significant features were observed

as described in the following sections.

Table 1. Measured geometric parameters of the 3D woven preform through µCT

Location Yarn Height(SD)

in mm

Width(SD) in mm

Intra-yarn fibre volume fraction

Number of measurements

Web warp(surface1_{) } _{0.32(±0.04) } _{1.72(±0.08) } _{46.30% } _{20 }

warp(internal2) 0.29(±0.02) 1.97(±0.08) 44.61% 50

weft(surface) 0.35(±0.03) 1.71(±0.07) 40.22% 20

weft(internal) 0.32(±0.03) 2.00(±0.13) 39.82% 50

(a)

warp & binder weft

weft

flange web

warp & binder weft

(b)

(c)

**Formatted:** Font:

## For Peer Review

Web crossover3

warp(surface) 0.22(±0.04) 1.81(±0.08) 64.00% 20

warp(internal) 0.17(±0.02) 2.02(±0.12) 74.21% 20

weft(surface) 0.30(±0.04) 1.65(±0.12) 51.48% 20

weft(internal) 0.19(±0.04) 1.87(±0.09) 71.73% 20

Flange warp(surface) 0.35(±0.04) 3.61(±0.14) 40.34% 20

warp(internal) 0.31(±0.03) 3.85(±0.08) 42.71% 20

Section

A-A weft layer1 0.28(±0.01) 2.63(±0.08) 34.61% 20

weft layer2 0.29(±0.03) 3.01(±0.11) 29.20% 20

weft layer5 0.29(±0.02) 3.57(±0.04) 24.62% 20

Spacing in the same layer (mm)

Spacing between through-thickness layers(mm)

warp 2.71(±0.03) 0.45(±0.10) 20

weft 3.33(±0.16) 0.44(±0.04) 20

1_{ surface yarns are those on the layers next to compaction fixture surfaces }
2

internal yarns are all other yarns except surface yarns

3

crossover refers to the locations where warp and weft yarns intersect

## Warp yarn shift

The first distinctive deformation is the shift of the warp yarn stack in the noodle regionat the junction, in

the direction orthogonal to the yarn length direction. The warp yarns within the same stack are aligned

vertically with each other before folding the preform, but their relative position is shifted after folding due

to the rigid body transformation in the noodle regionat the junction. However, the warp yarn shift could be

suppressed by the surrounding binder yarns.

The shift begins in the warp yarn stack at the bend as marked in Figure 3, and is followed by the next 1-2

stacks in the flange. It is noted from the µCT scan that this phenomenon is most evident in the noodle area,

and the level of shift reduces in the following stacks of warp yarns in the flange. To quantify the shift of the

warp yarn stack, shift in the bend can be represented by angle shift _{}, which is measured as the angle
between the two lines connecting centres of yarns to the normal direction of each yarn. Shift of the

**Formatted:** Font color: Red

**Formatted:** Font color: Red

## For Peer Review

[image:9.612.72.605.70.676.2]following stack is depicted as displacement shift _{} representing the horizontal distance between two yarn
centres as illustrated in Figure 3.

Figure 3. Warp yarn shift quantification in the noodle regionat the junction(weft yarns not shown); numbers show the numbering of warp layers

Warp yarn cross-section bending

Bent cross-sections of warp yarns were observed in the noodle regionat the junction. As shown in Figure 3,

each warp yarn bends about the centreline (or centre-plane) of its cross-section uniformly along its length

direction and its shape complies with the curvature of the adjacent weft yarn layers. For this 90° folded

preform, the centreline of each weft layer in the bend follows the path of a quarter of the circumference of a

circle. As a result, the centrelines of bent warp yarn cross-sections could be approximated with circular

paths of different radii. The measured radii of curvature of centrelines of bent warp cross-sections (_{}
in Figure 6) and weft yarn layers (_{} in Figure 5) are listed in Table 2.

Table 2. Measured and calculated radii of curvature of centrelines of bent warp yarn cross-sections and
weft yarn layers, here subscript *n* is the yarn layer number (mm; 5 measurements)

Measured values Calculated values (Eq.(1))

_{}_{}_{} _{}

_{ } _{}

Layer 1 2.19(±0.07) 2.38(±0.10) 2.18 2.4

Layer 2 2.42(±0.12) 2.78(±0.15) 2.62 2.84

Layer 3 3.11(±0.08) 3.11(±0.14) 3.06 3.28

Layer 4 3.63(±0.12) 3.71(±0.13) 3.5 3.72

Layer 5 4.25(±0.10) 3.94

## Weft yarn cross-section flattening

**Formatted:** Font: 10 pt, Font color: Red

**Formatted:** Font color: Red

For Peer Review

In Figure 4, section view A-A of Figure 2 shows the cross-sections of weft yarns at the middle of the bend

arc, while section B-B denotes sections of weft yarns in the flat region. It is obvious that the

cross-sections of weft yarns at section A-A are significantly flattened, i.e. an increase in yarn width and decease

in yarn height, especially for those not sitting in the peak or trough of the binder yarn path since here yarn

flattening is not constrained by binders. The cross-section data of flattened weft yarns without binder

constraint at position A-A were measured from the µCT scan and results are listed in Table 1. The layer

sequence of weft yarns in section A-A is numbered as Figure 2 shows. From further observation of µCT

images, the most slender cross-section of weft yarn occurs at position A-A in Figure 2, from where it

transitions symmetrically back to the dimension of the yarn cross-section in the flat part of the preform. It is

also observed that the length of yarn width transition varies for yarns on different layers, but all the

flattened yarns are of almost same height as shown in Table 1.

Meanwhile, a number of gaps in yarn cross-sections at section A-A were observed, which caused serrated

cross-section shapes in most of the weft yarns as marked in Figure 4. A number of different slices near

section A-A indicate this phenomenon and therefore it is unlikely to be an artefact of the µCT scan. The

position of each gap appears random as observed and the cross-sectional gap is simply quantified by its

maximum width that is named gap distance _{}. The value of _{} is no more than 1.5mm from several
measurements. The flattening and cross-sectional gaps of weft yarns at the bend partly result from fibre

migration when the preform is folded.15

Figure 4. µCT images showing weft yarn flattening (A-A: flattened; B-B: non-flattened); serrated cross-section shapes are marked in Section A-A

## Geometric modelling

For Peer Review

Warp yarn shifting

The warp yarn shift is inevitable due to the rigid body transformation in the noodle regionat the junction.

Each warp yarn has a different radius of curvature of cross-sectional centreline to the fillet origin *O*. As

illustrated in Figure 5, half of a flat piece of 3D woven preform (left) is folded to a 90° angle (right). _{#},

$ and % are the radii of curvature of centrelines for weft yarns on layer 1, 2 and 3 respectively. As

the radius of the inner surface of a T-piece is confined by the mould corner radius _{}, the following can be
obtained:

1

2 1

3 2

1

2

( ) / 2

*weft*

*weft* *weft*

*weft*

*weft*
*m*

*weft*

*weft*
*weft*

*warp*

*n* *n*

*w*
*n*
*eft* *weft*

*H*

*R* *R*

*R* *R* *D*

*R* *R* *D*

*R* *R* *R*+

= +

= +

= +

= +

(1)

where _{} is the height of the weft yarn; _{} is the spacing between through-thickness weft layers;

is the radius of curvature of centreline for the warp yarn cross-section on layer *n*.

Assuming there is no yarn sliding, angle shit _{} between warp yarn layer 1 and layer 2 (in radians) in
Figure 5 can be expressed as:

1 2 2 3 1 2

2( ) 2( ) 1 1

( )( )

*warp* *warp*

*warp*

*weft* *weft* *weft* *weft* *warp* *w r*
*o*

*a p*
*o*

*o*

*D* *D*

*S* *D*

*R* *R* *R* *R* *R*

*d*

*R*
*d*

*d*
θ

− −

= − = − −

+ + (2)

where _{} is the warp yarn spacing within the same layer, and _{} the offset distance from the centre of
nearest unbent weft yarn describing the position where the weft yarns start to bend; therefore _{}− _{}
denotes the arc length in between bending onset position and bent yarn centre along the bend.

**Formatted:** Font color: Red

### Field Code Changed

**Field Code Changed**

## For Peer Review

Figure 5. Schematic view of warp yarn shift due to rigid body transformation

Also, the displacement shift _{} in adjacent layers for the following stacks of weft yarns can be described as:

2 3 1 2

( )

2 2 2 2

*weft* *weft* *weft* *weft*

*d* *weft*

*R* *R* *R* *R*

*S* =π + − + =π*D* (3)

Warp yarn cross-section bending

Yarn cross-section shapes have been approximated by a number of researchers by elliptical, power

elliptical and lenticular shapes which can be defined by parametric equations in two dimensions.19

Therefore it is convenient to model the cross-section deformation by a parameterized transformation that

can apply to every current parametric cross-section shape rather than defining a new description for a

curved cross-section. The cross-section of one warp yarn is presented in Figure 6 prior to and after

deformation, where x and y represent the original yarn width and yarn height directions, and the origin is at

the yarn centre. Accordingly the x and y coordinates of the original cross-section (the dashed line in Figure

6) can be defined by:

( ) ( ) 0 t 2 ( ) ( ) 0 t 2

*x*

*y*
*C t* *f t*
*C t* *q t*

π π

= ≤ ≤

= ≤ ≤ (4)

" '

(

warp yarn

weft yarn 1 2 3

1!*+

2!*+ _{}
3
!*+

. 1

2 3

x y

o

!*+

/

### Field Code Changed

**Field Code Changed**

## For Peer Review

Figure 6. Schematic view of warp yarn cross-section bendingIt is assumed that the bent shape is a result of a simple conformation of the major axis from the axis *x* to the

arc in radius _{}0 (Eq.(1)). Thus, for each point on the upper half of the edge of a bent cross-section, the
transformation can be achieved by adding (∆x, ∆y) to the coordinates of corresponding points on the

original cross-section, where ∆x, ∆y can be defined by:

( )

( / 2) sin( ) ( )

/ 2 ( )

( / 2)(1 cos( ))

/ 2

*warp* *x*

*n* *warp* *warp* *x*

*n* *warp*

*warp* *x*

*n* *warp* *warp*

*n* *warp*
*C t*

*x* *R* *H* *C t*

*R* *H*

*C t*

*y* *R* *H*

*R* *H*
∆ = − −
−
∆ = − −
−
(5)

where _{} is the height of the warp yarn. Similarly, for the point on the lower half of the edge of a bent
cross-section, ∆x, ∆y are given by:

( )

( / 2) sin( ) ( )

/ 2 ( )

( / 2)(1 cos( ))

/ 2

*warp* *x*

*n* *warp* *warp* *x*

*n* *warp*

*warp* *x*

*n* *warp* *warp*

*n* *warp*
*C t*

*x* *R* *H* *C t*

*R* *H*

*C t*

*y* *R* *H*

*R* *H*
∆ = + −
+
∆ = + −
+
(6)

Usually the value of _{}/2 is quite small compared with _{}0, thus the above equations can be
simplified into one transformation for all the points on the cross-section:

( )

sin( ) ( )

( ) (1 cos( ))

*warp* *x*

*n* *warp* *x*

*n*

*warp* *x*

*n* *warp*

*n*

*C t*

*x* *R* *C t*

*R*
*C t*
*y* *R*
*R*
∆ = −
∆ = −
(7)

## Weft yarn cross-section flattening

∆y∆x x

y

2" '

warp yarn

weft yarn

### Field Code Changed

**Field Code Changed**

**Field Code Changed**

## For Peer Review

As shown in Figure 5 for half of a T-joint, each weft yarn is under a bending load. An idealized fibre

distribution in the weft yarn would consist of parallel layers with concentric arcs whose arc lengths are

dependent on each layer’s radial position. For illustration, Figure 7 represents a multi-filament yarn by

inner, middle and outer fibres/layers.

The model assumes that a fibre with high stiffness, such as carbon or glass fibre, has negligible axial

deformation in a bent yarn. After folding a straight yarn (Figure 7(a)), it is clear that the assumed fibre

arrangement in Figure 7(b) would lead to a fibre length difference which would not be realistic, in order to

satisfy the boundary condition that a fibre bundle is undisturbed beyond the bending location. Meanwhile,

Figure 7(c) shows another scenario where a fibre bundle with constant length complies with a 90o _{bend }

resulting in fibre ends at a sheared angle, which contradicts the real boundary condition. Therefore, to

maintain constant fibre length at a localised 90° bend, fibres tend to migrate and rearrange resulting in a

flattened yarn cross-section as observed in Figure 4.

Taking the outermost layer of fibres in Figure 7(b) as a reference line for fibre movement, the rest of the

fibres have to migrate to maintain their lengths. The positions of fibres except the reference ones in Figure

7(b) are considered as base positions for the movement. Hence the length differences between fibre on a

specific fibre layer and fibre on the reference layer can be expressed as:

2

*d*

*L* =π *d* (8)

where *d* is the distance from a specific fibre layer within the yarn to the reference layer. In practice,* d* can

be a series of discrete values depending on the fibre arrangement within the yarn.

Figure 7. Idealized fibre arrangement in a 90° bent yarn

### Field Code Changed

[image:14.612.134.393.498.631.2]## For Peer Review

There are two possible mechanisms for a fibre to migrate that maintains fibre length at a bending corner.

One mechanism is to move in the yarn height direction, referred to as in-plane migration (i.e. in the *x-y*

plane shown in Figure 8). The other way is to move in the yarn width direction, referred to as out-of-plane

migration (*z* direction in Figure 9). In-plane fibre migration will result in a reduction of yarn height while

out-of-plane migration will increase the yarn width.

## In-plane fibre migration

A reference fibre and a fibre on a neighbouring layer before and after migration are shown in Figure 8. The

fibre loci in the bend can be approximated by circular paths as shown in Figure 3, thus in this model each

[image:15.612.65.609.69.720.2]single fibre path is described by one quadrant and two tangential straight lines, such as _{}, _{} and _{3} in
Figure 8 for example(where script *0* or *d* refers to reference or neighbouring layer). The positions of the

two tangent straight lines are assumed to be fixed in migration based on the µCT observation that weft yarn

height is almost unchanged in the region away from the bend. According to the length relation in two axial

directions shown in Figure 8, the following expressions can be obtained:

+ = + + (9)

3+ = 3+ + (10)

where _{} is the radius of curvature of the reference fibre that can be expressed by the sum of radius of
curvature of yarn centreline and half of the flattened yarn height; _{} is radius of curvature of the fibre that
is distance *d* away from the reference fibre.

If a proportion *α* of the above defined arc length difference as shown in Eq.(8) is compensated by in-plane

fibre migration, the arc length difference between migrated and base fibres is 6/2. Thus the relation
between the length of the reference fibre and a migrated fibre on a layer distance *d* away can be given as:

+6_{2 }+ 3= +6_{2 }+ 3+ (1 − ) (11)

### Field Code Changed

**Field Code Changed**

**Field Code Changed**

## For Peer Review

Figure 8. Schematic view of in-plane fibre migration

Hence, the in-plane path of a migrated fibre at distance *d* away from the reference fibre is described by:

= − −_{4 − 6}6

= +_{4 − 6}6

3= 3+_{4 − 6}6 (12)

Out-of-plane fibre migration

Since a proportion *α* of the defined fibre length difference is compensated by in-plane fibre rearrangement,

the rest of the length difference, i.e. *(1-α)* of the whole length difference, has to be compensated by

out-of-plane fibre migration to meet the assumption that the folding process would not increase the arc length of

each fibre within a 90° bent yarn. In theory fibres can migrate in both directions across the yarn width.

In Figure 9, *LABCD* is the arc of a fibre which had in-plane but no out-of-plane migration so that its arc

length is given by:

:;<== + > + > = 2(− ) +6_{2 } (13)

where _{} is the length of yarn width transition, denoted by length between A(or D) and G, from where the
yarn width starts to change.

"0 _{ }

@0

@

0

reference fibre

migrated fibre

base fibre

x y

### Field Code Changed

**Field Code Changed**

## For Peer Review

Figure 9. Schematic view of out-of-plane fibre migration

To calculate the arc length of a post-migration fibre *LAEFD*, it is assumed that its radius of curvature is still

the same as *LABCD*. denotes the distance that the fibre has migrated laterally, therefore in ∆ we can

have:

sin$/

2 = ( 2⁄ )$ (14)

Also, in ∆ and ∆ we can have:

$= $+ $; $= $+ $ (15)

Hence, Eq.(14)(14) is given by:

sin$/

2 = 1 2 $

$+ $

(16)

where for simplicity _{} equals or ; equals .
From trigonometry we can say that:

tan$/

2 =

$

$+ 2$

(17)

Hence, in ∆IJI is given by:

I = IJ tan /2=

tan /2 (18)

The arc length of migrated fibre* LAEFD* is:

>

I K

I

K

J /

x y

z

### Field Code Changed

**Field Code Changed**

**Formatted:** Font:

**Field Code Changed**

**Field Code Changed**

**Field Code Changed**

## For Peer Review

:LM== I + IK + K

= 2(N$+ $−O
$_{+ 2}$

) + (6 − 2 tan
P#_{(} $

$+ 2$))

(19)

Thus, the relation between fibre arc length differences caused by out-of-plane fibre migration can be

represented by:

:LM=− :;<== (1 − ) (20)

Substituting Eq.(13)(13) and Eq.(19)(19) into Eq.(20)(20), the displacement for out-of-plane migration *w*

can be obtained for a fibre at a distance *d* away from the reference fibre.

## Yarn cross-section

The process of fibre migration resulting from bending is complex, as each single fibre may have a different

value of *α* for its in-plane and out-of-plane migrations. Ideally, if all fibres on the same layer move with the

same *α* and direction for out-of-plane migration, the cross-section of a weft yarn, assuming a square array

for fibre packing, at Section A-A in Figure 2 would have a parallelogram shape as shown in Figure 10(b),

where Figure 10(a) is the fibre arrangement before flattening with its left-hand layer as reference for

in-plane migration (Figure 8). Since there are thousands of fibres in a single yarn, a large number of fibres

presumably might migrate uniformly in the above way, i.e. without a change to their initial relative spatial

sequence, as shown for the fibres represented by black dots in Figure 10(c) which remain in their ideal

positions as in Figure 10(b). Meanwhile, a few fibres, not following the above ideal migration law, can

penetrate into a position out of their own layers through more in-plane migration once out-of-plane

migration of fibres on prior layers makes a space, as indicated by grey dots in Figure 10(c), which can

cause a random serrated section shape as observed in Figure 4. Additionally, a second possible

cross-section shape is shown in Figure 10(d) if it is assumed fibres move with the same *α* but in both directions

for out-of-plane migration. Hereafter the first large group of fibres following the pre-migration relative

spatial sequence are named ideally migrated fibres, and the second small group are called randomly

migrated fibres. Under this assumption, the values of *α* for the ideally migrated fibres are supposed to be

identically denoted by . Therefore the yarn height could be characterised by the distance between two corresponding fibres on the outermost layer(reference) and on the innermost layer respectively as shown in

Figure 11.

### Field Code Changed

**Field Code Changed**

**Formatted:** Font:

**Formatted:** Font:

**Formatted:** Font:

## For Peer Review

Figure 10. Schematic cross-section of fibre arrangement for a weft yarn showing fibre migration
mechanisms: (a) pre-migration, square packing fibre arrangement; (b) post-migration, idealized migration;
(c) and (d) post-migration, possible realistic migration accounting for serrated cross-section shape
If the flattened yarn height (at Section A-A in Figure 2) can be measured from a µCT scan, the value of * *

for ideally migrated fibres on the innermost layer could be calculated by solving the following equation

after substituting _{}_{QRS} with Eq.(12)(12):

max

0 2

*fla*

*weft* *d*

*H* =*R* −*R* − *dx* (21)

where _{} is the maximum value of *d *which is the original yarn height; (−*dx*, −*dy*) in Figure 11 is the
position of the centre of curvature of a fibre on the innermost layer in the coordinate system of reference

fibre with its centre of curvature as origin, which is given by:

max

0 *d* max

dx

=

dy

=

R

−

R

−

d

_{ }

_{(22) }

The yarn width is determined by the fibres that had out-of-plane migration. Irrespective of randomly

migrated fibres and considering all fibres to be ideal ones migrating in the yarn width direction with an

identical , the relative migration displacement *w* could be obtained by solving a combination of
Eq.(13)(13), (19)(19) and (20)(20). In this case, if the yarn extension, defined as the area beyond its

original cross-section (area of fibres outside of the dotted rectangle in Figure 10(b)), for the flattened yarn

is full of ideally migrated fibres, the total fibre area for fibres in the yarn extension can be roughly

estimated by:

= =

∑

ext
1
*f*

*n*

*k* *f*
*k*

*Area* *w d* (23)

**Formatted:** Font:

### Field Code Changed

**Field Code Changed**

**Formatted:** Font:

**Formatted:** Font:

**Formatted:** Font:

**Field Code Changed**

## For Peer Review

where _{} is the fibre diameter and *nf* is the number of total fibre layers along the yarn height direction

before flattening; _{} is the displacement of out-of-plane migration for a fibre on layer *k*.

Figure 11. Yarn in-plane section view (*=0.4; dmax=0.35*)

In reality, ideally migrated and randomly migrated fibres coexist in a bent yarn so that a flattened

cross-section can be near to rectangular with the observed gap (Figure 4) rather than a parallelogram (Figure 10

(b)) if all fibres are considered ideally migrated fibres. Some of the fibres, namely randomly migrated

fibres, in the yarn extension do not have to move that much in the yarn width direction because there is

enough space ahead of them to accommodate in-plane migration in the yarn height direction, in the

meantime the bending force will prioritise in-plane migration. Therefore a rectangular cross-section is

likely to be formed, and a rough prediction of weft yarn width extension *ext*
*weft*

*W* in terms of constant fibre

area in the yarn extension can be made by:

e x t /

*e x t* *fla*

*w e ft* *w e ft*

*W* = *A re a* *H* (24)

where the value of *fla*
*weft*

*H* should be known in advance.

However, it is not possible that different fibres on the same layer can move in both directions

simultaneously for out-of-plane migration as shown in Figure 10(d), because the measured _{} is much
smaller than double the value of maximum _{} as calculated in the following section. Hence the predicted
flattened yarn width can be expressed as:

*fla* *ext*

*w eft* *w eft* *weft*

*W* =*W* +*W* (25)

where _{} is the original weft yarn width. This model is capable to predict the change of yarn
cross-section if *fla*

*weft*

*H* can be determined.

."T

0

U

56/4

(−dx, −dy) T [

innermost layer/fibre middle layer/fibre outermost layer/fibre

### Field Code Changed

**Field Code Changed**

## For Peer Review

Validation

Three proposed models for warp yarn shifting, cross-section bending and weft yarn cross-section flattening

were compared to experimental data from the standard orthogonal weave region of the preform as listed in

Table 1.

Warp yarn shifting

The value of _{} is 2mm which equals the radius at the junction of the acrylic fixture contacting the
preform. Based on Eq.(1)(1), the radii of curvature of centrelines for warp cross-sections and weft yarns on

different yarn layers can be obtained as listed in Table 2, which shows good agreement with the measured

values.

The offset distance _{} for the preform is measured as 2.0mm and thus the relative angle shift of a warp
yarn can be derived by Eq.(2). Furthermore, the displacement shift in adjacent layers can be determined by

Eq.(3)(3). Since the yarn shift is not significant for this preform, the angle shit measurements were only

taken between yarns on layer 1 and yarns on other layers, whilst the displacement shift measurements were

carried out between yarns on layer 2 and 3, as numbered in Figure 3. The warp yarns shift in a uniform

manner but show a deviation along the yarn length direction. The measured shift values taken at different

cross-sections along the length direction with standard deviations are shown in Table 3 in comparison with

predicted values.

It is noticed that the measured angle shit between layer 1 and 3 is negative, which means the warp yarn on

layer 3 has slid to the flange while folding. Also it is the same with displacement shit for yarns on layer 1

and 4 in the next warp stack.

Table 3. Warp yarn shift measured and predicted results (10 measurements)

Angle shift (°)between Displacement shift (mm) between layer 2 and 3 layer 1 and 2 layer 1 and 3 layer 1 and 4

Measured value 2.96(±0.23) -1.48(±0.17) 6.48(±0.25) 0.87(±0.13)

Predicted value 2.63 4.55 6.01 0.69

Warp yarn stack shift can be observed but the trend does not always agree closely with the model since

binder yarns influence the movement of warp yarns as well as yarn sliding induced by the weaving process.

**Formatted:** Font:

**Formatted:** Font:

## For Peer Review

Warp yarn cross-section bending

A bent cross-section shape can be obtained by the transformation defined in Eq.(7) on the basis of an

original parameterized cross-section description. Figure 12(a) is based on an elliptical cross-section and its

radius of curvature of centreline is 3mm; Figure 12(b) is transformed from a super-ellipse (Eq.(26)) with

m=0.4 where radius of curvature of centreline of bent yarn cross-section is 2.4mm.

(a) elliptical cross-section (b) super-elliptical cross-section

Figure 12. Transformation of bent yarn cross-section shapes: dashed lines for original shapes and solid lines for bent shapes

It is observed that a real warp cross-section shape for this preform in the flat region can be better

approximated with a super-ellipse than an ellipse, thus validation of warp yarn bending is based on the

cross-section function for super-ellipse (m=0.4) with yarn height and width measured from the unbent

region in the web, where Eq. (4) can be expressed as:

( ) cos(t) 0 t 2

2

sin ( ) 0 t

2 ( )

( sin( )) t 2

2

*warp*
*x*

*warp* *m*

*y*

*warp* *m*

*W*
*C t*

*H*

*t*
*C t*

*H*

*t*

π

π

π π

= ≤ ≤

≤ ≤

=

− − ≤ ≤

(26)

Then the bent cross-sections for different radii of curvature can be plotted and compared with real yarns as

shown in Figure 13. The modelled cross-section gives good agreement with realistic bent cross-section

shapes.

-1.5 -1 -0.5 0 0.5 1 1.5

-1.5 -1 -0.5 0 0.5 1 1.5

-1.5 -1 -0.5 0 0.5 1 1.5

-1.5 -1 -0.5 0 0.5 1 1.5

### Field Code Changed

## For Peer Review

Figure 13. Model produced cross-section shapes in comparison with real yarnsWeft yarn cross-section flattening

Validation of cross-section flattening was carried out for yarns on three different layers in order to cover

the full radius of curvature values which are the most essential parameters in yarn bending. The three layers

selected are layer 1, 2 and 5 in section A-A of Figure 4. Weft yarn cross-section transition length _{} is
obtained from measurement for each layer, and radius of curvature of the reference fibre _{} is derived
based on calculated radius of curvature yarn centreline and flattened yarn height.

The total number of fibre layers along the yarn height direction before flattening *nf* (Eq.(23)(23)) is

estimated based on yarn dimensions before flattening and filament count as well as the assumption that the

cross-section was a rectangular shape with square fibre packing. Based on the flattened yarn height, can be obtainedby solving a combination of Eq.(12)(12), (21) and (22). Then the displacement of fibre

out-of-plane migration along the yarn height if all the fibres are ideally migrated ones can be obtained by solving a

combination of Eq.(13)(13), (19)(19) and (20)(20) as plotted in Figure 14. Yarn extension width can be

calculated from Eq.(23) and (24), and all the parameters for the prediction model are listed in Table 4.

Table 4. Parameters for the yarn flattening prediction model

(mm) 10 measurements

(mm)

* *

(-)

*dmax *

(mm)

*nf *

(-)

(mm)

U (mm)

Yarn on layer 1 4.54(±0.18) 2.32 0.132 0.35 50 1.22 2.93

Yarn on layer 2 4.86(±0.16) 2.77 0.062 0.32 44 1.15 3.15

Yarn on layer 5 6.31(±0.14) 4.09 0.062 0.32 44 1.46 3.46

x y

**Formatted:** Font:

**Formatted:** Font:

**Formatted:** Font:

**Formatted:** Font:

**Formatted:** Font:

## For Peer Review

Figure 14. Relative displacement for fibre out-of-plane migrationFurthermore, the measured yarn width and predicted yarn width for the flattened weft yarns are compared

in Figure 15 and reasonable agreement is observed.

Figure 15. Comparison of measured and predicted yarn width for weft yarns

Although the prediction accuracy is good, the model is semi-empirical based on the input parameters of

flattened yarn height and cross-section transition length. However it is interesting that all the flattened weft

yarns with different radii of curvature have nearly the same height while the length over which

cross-section transitions occur seems to increase linearly with radius of curvature in bending, both of which are

merit further investigation.

## Conclusions

0 0.1 0.2 0.3

0 0.5 1 1.5 2 2.5 3

d/mm

w

/m

m

yarn on layer 1 yarn on layer 2 yarn on layer 5

2.93

3.15

3.46

2.63±0.08

3.01±0.11

3.57±0.04

1.5 2 2.5 3 3.5 4

Yarn on layer 1 Yarn on layer 2 Yarn on layer 5

fl

at

te

n

ed

y

ar

n

w

id

th

/m

m

Predicted

Measured

7

For Peer Review

To characterise the relationship between the fibre architecture and composite mechanical performance, a

numerical simulation requires a realistic geometric model as input. In this study, three geometric features,

yarn shifting, cross-section bending and flattening, caused by the bifurcation of a 3D flat woven preform

for composite T-joints were identified by µCT analysis and approximated analytically. A simple model

based on rigid body movement was used to approximate warp yarn shifting but the experimentally

observed trend does not always agree closely with the model. The model would benefit from considering

the influence of binder yarns on movement of warp yarns as well as yarn sliding induced by the weaving

process but this would complicate the model significantly. Yarn cross-section bending was modelled by a

transformation of the existing parameterized description of cross-section shape instead of proposing a new

shape function, and good agreement was obtained when compared with µCT results. Lastly, weft yarn

flattening was described in detail and a semi-empirical model was developed to predict the flattened yarn

width and satisfactory agreement with experiments was observed. However, it is worthwhile to further

study the preform compaction behaviour and form a fully predictive model for yarn flattening.

## Declaration of Conflicting Interests

The authors declare that there is no conflict of interest.

Funding

This work was supported by the Engineering and Physical Sciences Research Council (EPSRC), United

Kingdom [grant number: EP/IO33513/1], through the EPSRC Centre for Innovative Manufacturing in

Composites.

References

1. Bilisik K. Multiaxis three-dimensional weaving for composites: A review.

## Text Res J

2012; 82: 725-743.

2. Cartié DDR, Dell’Anno G, Poulin E, et al. 3D reinforcement of stiffener-to-skin

T-joints by Z-pinning and tufting.

Eng Fract Mech

2006; 73: 2532-2540.

For Peer Review

3. Koh TM, Feih S and Mouritz AP. Strengthening mechanics of thin and thick

composite T-joints reinforced with z-pins.

## Composites Part A

2012; 43: 1308-1317.

4. Soden JA, Weissenbach G and Hill BJ. The design and fabrication of 3D multi-layer

woven T-section reinforcements.

Composites Part A

1999; 30: 213-220.

5. Chiu CH and Cheng CC. Weaving Method of 3D Woven Preforms for Advanced

Composite Materials.

Text Res J

2003; 73: 37-41.

6. Fazeli M, Hübner M, Lehmann T, et al. Development of seamless woven node

## element structures for application in integral constructions.

Text Res J

2015; 86:

1220-1227.

7. Fazeli M, Kern M, Hoffmann G, et al. Development of three-dimensional profiled

woven fabrics on narrow fabric looms.

Text Res J

2015; 86: 1328-1340.

8. Khokar N. 3D-weaving: Theory and practice.

J Text Inst

2001; 92: 193-207.

9. Amirul I. 3D woven structures and an overview of manufacturing techniques. In:

4th

World Conference on 3D Fabrics and Their Applications

## , Aachen, Germany, 2012.

10. Chen X, Taylor LW and Tsai LJ. An overview on fabrication of three-dimensional

woven textile preforms for composites.

Text Res J

2011; 81: 932-944.

11. Thomson RS, Falzon PJ, Nicolaidis A, et al. The bending properties of integrally

woven and unidirectional prepreg T-sections.

Compos Struct

1999; 47: 781-787.

12. Mouritz AP and Cox BN. A mechanistic interpretation of the comparative in-plane

## mechanical properties of 3D woven, stitched and pinned composites.

Composites

Part A

2010; 41: 709-728.

13. Endruweit A, McGregor P, Long AC, et al. Influence of the fabric architecture on the

variations in experimentally determined in-plane permeability values.

Compos Sci

Technol

2006; 66: 1778-1792.

For Peer Review

14. Skordos AA and Sutcliffe MPF. Stochastic simulation of woven composites forming.

Compos Sci Technol

2008; 68: 283-296.

## 15. Fast T, Scott AE, Bale HA, et al. Topological and Euclidean metrics reveal spatially

nonuniform structure in the entanglement of stochastic fiber bundles.

J Mater Sci

2015; 50: 2370-2398.

16. Yan S, Long A and Zeng X. Experimental assessment and numerical analysis of 3D

woven composite T-joints under tensile loading. In:

Proceedings of the 20th

International Conference on Composite Materials (ICCM 20)

, Copenhagen,

Denmark, 2015.

## 17. Desplentere F, Lomov SV, Woerdeman DL, et al. Micro-CT characterization of

variability in 3D textile architecture.

Compos Sci Technol

2005; 65: 1920-1930.

18. Karahan M, Lomov SV, Bogdanovich AE, et al. Internal geometry evaluation of

non-crimp 3D orthogonal woven carbon fabric composite.

Composites Part A

2010;

41: 1301-1311.

19. Sherburn M.

Geometric and Mechanical Modelling of Textiles

. PhD Thesis,

University of Nottingham, UK, 2007.

## 20. Lin H, Brown LP and Long AC. Modelling and Simulating Textile Structures Using

TexGen.

Adv Mat Res

2011; 331: 44-47.

21. Stig F and Hallstrom S. Spatial modelling of 3D-woven textiles.

Compos Struct

2012; 94: 1495-1502.

22. Lomov SV, Gusakov AV, Huysmans G, et al. Textile geometry preprocessor for

meso-mechanical models of woven composites.

Compos Sci Technol

2000; 60:

2083-2095.

23. Mahadik Y and Hallett SR. Finite element modelling of tow geometry in 3D woven

## fabrics.

Composites Part A

2010; 41: 1192-1200.

For Peer Review

24. Zhou G, Sun X and Wang Y. Multi-chain digital element analysis in textile

mechanics.

Compos Sci Technol

2004; 64: 239-244.

25. Lomov SV and Verpoest I. Compression of woven reinforcements: A mathematical

model.

J Reinf Plast Compos

2000; 19: 1329-1350.

26. Chen ZR, Ye L and Kruckenberg T. A micromechanical compaction model for

## woven fabric preforms. Part I: Single layer.

Compos Sci Technol

2006; 66:

3254-3262.

27. Chen ZR and Ye L. A micromechanical compaction model for woven fabric

preforms. Part II: Multilayer.

Compos Sci Technol

2006; 66: 3263-3272.

28. Cornelissen B and Akkerman R. Analysis of yarn bending behaviour. In:

Proceedings of the 17th International Conference on Composite Materials (ICCM

17)